Angew Chem Int Ed_Crystal Engg_A Holistic View_Desiraju_2007
Embed Size (px)
Transcript of Angew Chem Int Ed_Crystal Engg_A Holistic View_Desiraju_2007
G. R. Desiraju
Crystal Engineering: A Holistic ViewGautam R. Desiraju*
Keywords: crystal engineering hydrogen bonds intermolecular interactions polymorphism supramolecular chemistry
Chemie 2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim Angew. Chem. Int. Ed. 2007, 46, 8342 8356
Crystal engineering, the design of molecular solids, is the synthesis offunctional solid-state structures from neutral or ionic building blocks, using intermolecular interactions in the design strategy. Hydrogen bonds, coordination bonds, and other less directed interactions define substructural patterns, referred to in the literature as supramolecular synthons and secondary building units. Crystal engineering has considerable overlap with supramolecular chemistry, X-ray crystallography, materials science, and solid-state chemistry and yet it is a distinct discipline in itself. The subject goes beyond the traditional divisions of organic, inorganic, and physical chemistry, and this makes for a very eclectic blend of ideas and techniques. The purpose of this Review is to highlight some current challenges in this rapidly evolving subject. Among the topics discussed are the nature of intermolecular interactions and their role in crystal design, the sometimes diverging perceptions of the geometrical and chemical models for a molecular crystal, the relationship of these models to polymorphism, knowledgebased computational prediction of crystal structures, and efforts at mapping the pathway of the crystallization reaction.
From the Contents1. Introduction 2. Crystal Design and Function 3. Intermolecular Interactions 4. Crystal Packing and Polymorphism. The Holistic Crystal 5. Crystal Structure Prediction (CSP) 6. Crystallization Mechanisms 7. Summary and Outlook 8343 8345 8347
8350 8351 8354
1. IntroductionCrystal engineering is the rational design of functional molecular solids. This subject is of both fundamental and practical interest to solid-state and structural chemists, and also important to those who attempt to design other kinds of organized phases and assemblies. In a broader sense, the concepts of crystal engineering are applicable to any kind of intermolecular assembly, for example, protein-ligand recognition. Crystal engineering is therefore of very wide scope and accordingly, it has brought together investigators from a variety of disciplines. The field has its origins in organic chemistry, more specifically organic solid-state photochemistry, and in physical chemistry, notably studies on the packing of molecular crystals, exemplified respectively by the contributions of G. M. J. Schmidt (19501970) and A. I. Kitaigorodskii (19401980). It gained an identity of sorts by the 1980s, attracting crystallographers, solid-state chemists, theoreticians, and inorganic chemists to its ranks. Today, the subject covers a community of at least 150 independent research groups, with two specialist journalsCrystal Growth and Design from the ACS and CrystEngComm from the RSCand even a dedicated webpage and a Wikipedia site maintained by the latter society. A working definition of crystal engineering, which I supplied in my 1989 book, namely that it is the understanding of intermolecular interactions in the context of crystal packing and in the utilisation of such understanding in the design of new solids with desired physical and chemical properties, seems to have stood the test of time, and the subject today includes three distinct activities, which form a continuous sequence: 1) the study of intermolecular interactions; 2) the study of packing modes, in the context of these interactions and with the aim of defining a design strategy; and 3) the study of crystal properAngew. Chem. Int. Ed. 2007, 46, 8342 8356
ties and their fine-tuning with deliberate variations in the packing. In effect, these three stages represent the what, how, and why of crystal engineering. With so many researchers approaching the subject from various independent and attractive viewpoints, individual opinions on what crystal engineering is and what it can do are bound to differ. Arguably, these differences have to do with style and taste. Fundamentally, however, there are two aspects of crystal engineering which are above debatethat it is a type of synthesis, and that a molecular crystal lends itself to the supramolecular paradigm. These ideas took root in the 1990s and need to be placed in the context of broader trends in the chemical sciences that occurred during that time.
1.1. Supramolecular Synthesis That a crystal can be viewed as a supramolecular entity follows from Lehns argument that a supermolecule is to the molecule as an intermolecular interaction is to the covalent bond, and it was Dunitz who first expressed this notion explicitlythe crystal is a supermolecule par excellence, and knowledge and control of intermolecular interactions is as vital to crystal synthesis as is control of the covalent bond is to molecular synthesis. The meaning and execution of synthesis in the supramolecular context were a parallel development in the mid-1990s, and three reviews are notable in this context. The first of these by Whitesides and co-workers appeared in early 1995 and explained the difference between
[*] Prof. Dr. G. R. Desiraju School of Chemistry, University of Hyderabad, Hyderabad 500 046 (India) Fax: (+ 91) 40-23010567 E-mail: [email protected] Homepage: http://18.104.22.168/ ~ grd/
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Reviewscovalent and supramolecular synthesis. The former is enthalpically controlled and products are often kinetic, while in the latter, the energies involved are much smaller and therefore the products reflect a balance between enthalpy and entropy. Implicit in this discussion is that the products are formed in solution in both processes. This is not the case in crystallization, a largely kinetic process, and in the second of these reviews, which appeared in late 1995, I put forward the concept of supramolecular synthons, kinetically defined structural units that ideally express the core features or kernel of a crystal structure, and which encapsulate the essence of the crystal in terms of molecular recognition. The synthon consists of molecular fragments and the supramolecular associations between them, and these associations need not be just hydrogen bonds and other directional interactions. An important, indeed critical, assumption is that the supramolecular synthon is a reasonable approximation to the entire crystal despite the simplification that is inherent in its definition. The third of these reviews, which followed in 1997, is aptly titled Synthetic Supramolecular Chemistry and in it, the authors Fyfe and Stoddart discuss processes both in solution and involving crystallization. While Whitesides and Stoddart generally considered zero-dimensional supramolecular objects as synthetic targets, my review focused exclusively on the crystal, which is a three-dimensional object. Attacking either of these types of target (zero-dimensional or higher-dimensional) has its own attractions and difficulties. Since the rest of this review will deal with crystals, it is not out of place to mention now the elegant strategies proposed for zero-dimensional supramolecular targets by Fujita,[33, 34] Stang, Raymond, Mirkin, and Stoddart, to name a few. In these cases, entropic considerations are of the greatest importance, and the supermolecule exists in solution before it gives a crystal, a necessary prerequisite perhaps for structural characterization, but crystallization is not implicated as a synthetic step.
G. R. Desiraju
1.2. Simplifying the Problem But what of the crystal? When one claims that a crystal is a supramolecular entity, one is admitting ipso facto that it is not possible to predict or directly anticipate the structure of aGautam R. Desiraju (born 1952, Madras, India; PhD, University of Illinois, 1976) has been associated, for over two decades, with the subject of crystal engineering and structural aspects of the hydrogen bond and other intermolecular interactions. He has authored two definitive books (Crystal Engineering: The Design of Organic Solids and The Weak Hydrogen Bond in Structural Chemistry and Biology) and is the recipient of several awards and recognitions including the Alexander von Humboldt Forschungspreis (2000) and the Third World Academy of Sciences Award in Chemistry (2000). He is a member of the editorial advisory boards of Chemistry An Asian Journal, Crystal Growth & Design, and CrystEngComm.
crystal from the structure of the constituent isolated molecule. The essence of supramolecular chemistry is that the structure and properties of the higher-level entities (supermolecules, crystals) cannot be predicted directly or immediately from those of the lower-level entities (molecules). Crystals represent a higher level of complexity than molecules, and crystal structure is accordingly an emergent property with crystallization being a supramolecular reaction. The main aim of crystal engineering is to construct crystal structures from molecular structures. This is the synthetic step, and it is not straightforward because of the emergent nature of the crystal structure. To develop a synthetic strategy, a retrosynthetic step is invoked which effectively simplifies the crystal structure to a smaller unit called the synthon. Let us consider a molecule to consist of several functionalities or functional groups (F1, F2, Fn) and during crystallization, these functionalities come together through a process of molecular recognition utilizing weak interactions to generate supramolecular synthons (S1, S2, Sn). The conjunction of particular supramolecular synthons uniquely defines any crystal structure. If the kinetic factors are sufficiently dominant, some synthons (say, S1, S3) may invariably occur when the molecules contain some specific functionalities (say, M2, M3, M5), whatever be the nature of the other molecular functionalities present. It is precisely this situation that the crystal engineer seeks, for then one can identify a series of related molecules which (through some conserved synthons) will give a series of related crystals. However, this is an ideal situation, and serious problems often arise in that no correspondence between molecular and crystal structure is easily perceived. This happens for several reasons: 1) the number of possible and competing supramolecular synthons can quickly become very large for a small increase in molecular functionality because all the intermolecular interactions are weak; 2) structural interference from remote molecular functionalities may be fickle and unpredictable; 3) the hydrocarbon core of an organic molecule, which is not generally considered to be a functional group in molecular chemistry, is very much a supramolecular functionality and will interfere regularly with other putative interactions from more polar residues. This final issue is perhaps the most difficult to handle. The crystal structures of the substituted phenylpropiolic acids illustrate the interference offered by remote functionalities. Carboxylic acids show either the common dimer or the rare catemer patterns in their crystals (Scheme 1). However, both catemers and dimers have two OHO hydrogen bonds for each carboxyl group, and so the reasons for the rarity of the catemer must lie elsewhere. A recent study from our group shows that the formation of the catemer is only possible if there is a supporting hydrogen bond (say, CHO) from another location on the molecule. This condition prevails in the family of substituted phenylpropiolic acids. When, why, and how this supporting interaction manifests itself is not easy to establish. We examined at least 30 to 40 crystal structures over a decade before we were able to draw some conclusions. In the end, however, understanding crystal structures is like pattern recognition. The larger the sampling of crystal structures examined, the greater the likelihood thatAngew. Chem. Int. Ed. 2007, 46, 8342 8356
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Angewandteto manipulate each set independently. Crystal design seems to have developed in two distinct ways, and these are best exemplified by the organics and the metalorganics; these categories differ in terms of ones ability to thus manipulate the structure. The main design problem with a pure organic crystal is that for a three-dimensional structure with comparable (and strong) interactions in the three directions, the molecular structure itself should be three-dimensional. This would tend to suggest aliphatic molecules, but not so much work has been done with this category of substance. The noteworthy exceptions are the organic diamondoid solids, the structures of which are inspired by Ermers prototype, adamantane1,3,5,7-tetracarboxylic acid with its fivefold interpenetration of open hydrogen-bonded networks. Open frameworks are advantageous in achieving microporous structures, and if they can be designed so as not to interpenetrate, then this property could become a reality. However, avoidance of interpenetration is difficult. Another disadvantage of these tetrahedral molecules is that they are functionally similar in all directions, and so independent and modular manipulation of functionality is a distant dream. We attempted some work in this direction. The tetraphenylmethane derivative 1 (Scheme 2) was made to ascertain if the NO2I synthon is robust enough that it can act as a connector in the generation of a diamondoid structure. If this were the case, the unsymmetrical substitution pattern in the molecule would introduce polarity in the crystal. The structure fulfilled our prediction (space group Fdd2) , but it is still interpenetrated, and the yields of the molecular precursor (in a six-step synthesis) were so low that this is a hardly a practicable method for general crystal engineering (Figure 1). Aromatic molecules have been studied extensively, but by their very nature, some intermolecular interactions (pp, C HO) in the crystal structure will be much weaker than others (for example, OHO and NHO hydrogen bonding) in different directions. Accordingly, two-dimensional structural control is easily achieved in the planes of the aromatic rings, but control in the third dimension is mostly elusive. The challenge here is to avoid structural interference from competing interactions. We examined a family of geminal alkynols, a group of compounds wherein the structural fidelity between related molecules is particularly poor because the two hydrogen bond donors (OH, CH) and two acceptors (OH, CC) are all in close proximity in the molecule and therefore sterically hindered. The resulting modifications in hydrogen bond donor and acceptor strengths make all the four possible hydrogen bonds (OHO, C HO, OHp, CHp) of comparable importance, leading to structural unpredictability. However, even in a fickle set of compounds such as this, we observed some structural consistency. For example, the crystal structures of the dimethyl derivative 2 (Scheme 2) and the anthracene derivative 3 are the same down to the level of fine details of hydrogen bonding (Figure 2). The methyl groups in 2 are surrogates of the annelated benzo residues in 3; indeed one may view them as vestigial benzene rings, and the characteristic cooperative chain of hydrogen bridges (OHOHC CHCCHOH) which forms an infinite pattern is www.angewandte.org
Scheme 1. Dimer (top) and catemer (bottom) structures in phenylpropiolic acids. Unlike other carboxylic acids, the catemer dominates in this family.
increasingly complex molecule!crystal algorithms will be decoded. It would seem that brute-force methods will eventually win.
1.3. Scope of this Review With this background, I would like to enumerate and briefly discuss some of the outstanding problems and challenges in crystal engineering today. This view is a subjective one, and a survey of all interesting and useful ongoing studies is neither practical nor possible in a subject that is currently undergoing a phase of explosive growth. Notably, much work is being undertaken in industry and academia on polymorphism,[42, 43] or the existence of multiple crystal forms of drugs and active pharmaceutical ingredients (APIs), especially with regard to the legal implications of such work, but the reader of this article will not find here a discussion of API polymorphism and the extension of pharmaceutical space through, say, the device of the so-called cocrystal formation. Undoubtedly, drug polymorphism has highlighted the importance of crystal engineering to a larger scientific audience, but there are more basic aspects to the study of polymorphism. This subject goes far beyond legal issues: It might offer the key to unlocking the mystery of crystallization.
2. Crystal Design and FunctionPredictability of crystal structure is the first step towards fine-tuning of properties. It is of little use if a given crystal structure is very sensitive to minor molecular changes because such changes would be required anyway in the optimization of the crystal properties. In an ideal situation, a crystal structure is held by sets of robust intermolecular interactions in roughly orthogonal directions, and the crystal engineer should be ableAngew. Chem. Int. Ed. 2007, 46, 8342 8356
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
G. R. Desiraju
Figure 1. Crystal engineering of a polar network. An unsymmetrically substituted tetraphenylmethane (in this case, a dinitro diiodo derivative) with a sufficiently robust heteroatom interaction (in this case, NO2I) will generate a polar crystal.
Scheme 2. Molecules and synthons discussed in this review.
conserved in both structures. These geminal alkynols show an unexpected level of three dimensionality in their crystal packing. The hydrogen bonds are arranged in a sheet while the aryl residues interdigitate in a perpendicular direction, and the isostructurality between the dimethyl and anthracene derivative is a consequence of interaction insulation between the hydrogen-bonded layers and the hydrocarbon residues. Interestingly, though, the crux of this structure is constituted with the tetrahedral C atom and the various interactions formed by the substituents at this positionand the C atom is aliphatic. All this is still quite far from functional crystals. The greatest opportunities in this direction possibly lie within the metalorganic framework (MOF) structures which are in themselves a part of a larger group of structures known as coordination polymers.[10, 5053] A polyvalent (transition-)metal ion acts as an effective multidimensional hub, from which emerge organic spokes that connect the hubs forming the three-dimensional structure. The distinction between coordi-
nation chemistry in general and coordination polymers in the context of crystal design and engineering was first made by Robson, who showed that because of the strength of the interactions, metalorganic compounds show a degree of structural modularity that is unknown in the pure organics. Rather quickly, strategies to avoid interpenetration were in place, and large framework structures were obtained. These large spatial voids could be used to contain guest molecules of various types. The so-called first-generation coordination polymers in which the host frameworks collapsed upon guest removal gave way to more sturdy second-generation compounds wherein the host framework is stable when evacuated. The work of Yaghi, in particular, on MOFs that can include large volumes of hydrogen is noteworthy. The challenge now is to make a MOF with a property (for example, hydrogen storage) which is industrially competitive and can lead to large-scale production. Third-generation compounds also have the aspect of function which is related to a flexible host framework. The work of Kitagawa and coworkers wherein a metalorganic solid is able to discriminate between acetylene and CO2, two molecules with nearly theAngew. Chem. Int. Ed. 2007, 46, 8342 8356
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Angewandtevarieties (organometallic,[65, 66] charge-assisted, blue-shifted) in routine crystal engineering. Molecular inorganic systems have also been studied; the well-known aurophilic AuAu interaction is described in a crystal engineering context. The uranyl group has also been mentioned. There is even an in silico design of a molecular quasicrystal. As far as intermolecular interactions are concerned, the last frontier in terms of grappling with them lies indubitably in understanding the supramolecular chemistry of the CF group, the so-called organic fluorine. Fluorine is so elecFigure 2. Isostructurality in dimethyl and anthracene geminal alkynols. The anthratronegative and nonpolarizable that it forms cene derivative 3 (left) forms a hydrogen-bonded sheet in the plane of the paper with nonbonding contacts only with great reluctance. the benzo rings pointing in and out of the plane. The same sheet is conserved in the Dunitz has pointed out that the CFHO dimethyl derivative 2 (right), and the methyl groups point up and down (A and B hydrogen bond is extremely rare. The CF refer to symmetry-independent molecules). In both cases, these 2D patterns group is not a good hydrogen bond acceptor like interdigitate with their orthogonally located hydrocarbon substituents. The cooperative hydrogen-bonded network is highlighted green in both parts. Synthons I and II the CNH2 and the COH groups, although F is are identical to 9 and 10 in Scheme 2. Note that I and II are conjoined in the same more electronegative than O and N. CFHC way in the two structures. contacts are very weak and seem to have hydrogen bond like characteristics only in compounds such as polyfluorinated benzenes wherein the acidity of the same shape and size, is of seminal importance.[57, 58] The host, CH groups is enhanced to levels which permit hydrogen which is originally collapsed, expands in contact with bonding, and there seems to be an adequate theoretical acetylene, which is absorbed rapidly. There is no similar affinity with CO2. Why do these two gases behave differently? basis for their viability. We do not know the nature of the putative FF interaction because fluorine is a very complex It is seen that the acetylene guest binds to the host with C HO hydrogen bonds by the end of the process; clearly these element in supramolecular terms. If one takes a hydrocarbon interactions are specific enough to bring about an expansion and successively replaces the H atoms by F atoms, the boiling of the host framework and concomitant entry of the guest. In point rises (as it is expected to) initially but then falls. For general, the role of CHO contacts in crystals has been example, the boiling point of methane and its fluorinated debated. Do they fulfill specific structure-directing roles, derivatives are as follows: CH4 (161.5 8C), CH3F (78.4 8C), or are they merely innocuous bystanders in the general CH2F2 (51.7 8C), CHF3 (82.2 8C), CF4 (128.0 8C). Such packing panorama? The above-mentioned example of Kitabehavior is not exhibited by the other halogens. For example, gawa shows that CHO interactions are specific and the boiling points of the corresponding chloromethanes are: attractive; they literally suck the acetylene molecules into CH3Cl (24.2 8C), CH2Cl2 (39.5 8C), CHCl3 (61.2 8C), CCl4 the host framework. (76.0 8C). No one has been able to explain this anomaly properly. Does this arise from some kind of FF repulsion? Fluorine effectively repels itself in crystals, and the work of Hulliger and Fourmigu reveals this effect adequately. 3. Intermolecular Interactions The element is also unusual in that the so-called fluorous compounds with many CF bonds (for example, teflon) are After metal-coordination bonds and ionic interactions, neither hydrophilic or hydrophobic. In the end, I am not the strongest interactions in crystal engineering are hydrogen bonds. They are also directionally specific, and this is sure what a van der Waals radius of (organic) fluorine distinctly advantageous in crystal design, wherein they are signifies, considering that the element does not form any widely used. Robertsons criterion of maximum hydrogen intermolecular contacts of note with any other element. The bonding seems to be followed almost invariably with understanding of organic fluorine is one of the big challenges in crystal engineering. Success in this area might multifurcation and hydration being employed to fulfill the well lead to industrial spin-offs, and there are biological hydrogen bond capabilities of all donors and acceptors. In small organic molecules the acceptors are generally in excess implications as well in the drug design area, as noted by of the donors, and so free XH groups are extremely rare. Diederich. The converse is true incidentally in macromolecular structures in which the donors (if CH groups are included) outnumber the acceptors; as a result, any available acceptor is 4. Crystal Packing and Polymorphism. The Holistic used, including p rings, accounting for a higher incidence of, Crystal for example, XHp interactions. Hydrogen bonding is by now so well understood that there seems to be little to learn The packing of organic molecular crystals will now be that is startlingly new about the interaction itself.[59, 60, 64] What considered from two different viewpoints. The original approach is based on geometry and goes back to Kitaigoris largely unexplored is the use of some of the more exoticAngew. Chem. Int. Ed. 2007, 46, 8342 8356 2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
G. R. Desiraju
Figure 3. Thermodynamic and kinetic outcomes of crystallization (reproduced with permission from reference ).
odskii. Interactions between molecules are assumed to be weak and lacking in directionality; it is further assumed that all interactions taper off at longer distances in roughly the same way. In this isotropic model, crystal structures are governed by close packing. The structure that makes the most economical use of space is the best one, and molecules crystallize so that the bumps in the surface of one molecule fit into the hollows in the surface of the other. The 6-exp potential (or its variants), which is commonly used to describe such a situation, implies long-range attractions and shortrange repulsions, which effectively determine molecular shape. This model generally does not assign any significant role to directional intermolecular interactions, and has been advocated in recent times by Dunitz and Gavezzotti, who have presented a number of crystal structures wherein overall close packing rather than specific interactions seems to be the critical determinant. Kitaigorodskii himself was guarded on the role of hydrogen bonding and donoracceptor interactions in crystal structures. In reality, however, hydrogen bonding is quite important in crystals; molecules that have functional groups which can form hydrogen bonds almost always prefer to use these groups in such interactions. As hydrogen bonds become weaker, the anisotropic component in the packing decreases, but it never goes away entirely. One can model these interactions with electrostatic terms within a standard set of empirical isotropic potentials, but this will only provide an approximate description of a molecular crystal. Kitaigorodskii was not ashamed about this. He said that it is better to have a rough theory for all crystals rather than a fine theory that would be applicable only to benzene and urotropin. He added (in a later work) that atom potentials were not even required to describe crystal packing. But many decades have elapsed since he wrote this. Can we do better today? A crystal may alternatively be considered on the basis of chemical factors, in other words on the basis of directional interactions formed by the heteroatoms. In a major simplification, one might assume that it is sufficient to look just at strong hydrogen bonds like NHO and OHO. Indeed, one could simplify this even further and state that the hydrogen bond between the best hydrogen bond donor and the best acceptor is the most significant interaction in the
crystal, and that it will form typically. This model was originally proposed by Etter and calls for a hierarchy of hydrogen bonds: The donors and acceptors pair off in order of strength, and crystal structures can hopefully be understood on this basis. Empirical rules for hydrogen bonding in crystals were proposed, which included specific rules for specific functional groups, and examples that satisfied such rules were reported. However, exceptions are common, and other examples which do not follow the hierarchic model have also been published. In retrospect, much of this should be taken as guidelines rather than as formal rules, and todays exceptions become tomorrows rules as the number and variety of crystal structure determinations increase. Indeed, this was acknowledged by Etter, who noted that the rules should evolve as new structures become available. Notably, in the context of polymorphic compounds, there are lesser chances of adherence to interaction hierarchy in some of the polymorphs. To summarize, one notes that as the subject of crystal engineering has grown in breadth and scope, a very large number of crystal structures have been designed using the principles of hydrogen bonding. The geometrical approach (lack of structural directionality) relies on energy-landscape scenarios in discriminating between potential structures while the chemical approach (structural directionality brought about by chemical factors) requires a real-space examination of molecular features to select a packing direction. The supramolecular synthon concept provides a middle ground between these approaches because a synthon includes elements of both geometrical and chemical recognition. In this sense, the synthon concept is a more holistic approach to understanding molecular crystals. An oblate molecule packs with shape (geometrical recognition) as a structure director while an interaction direction (chemical recognition) leads eventually to close packing. Consider the prototype structure, benzene. Does one term it a close-packed structure based on the herringbone geometry, or is the herringbone geometry derived from a directional C Hp hydrogen bond? To conclude, the reader should note that the geometrical and chemical approaches do not necessarily negate each other.
4.1. Thermodynamic and Kinetic Crystallization At their idealized extremes, the geometrical and chemical models seem to be contradictory. In the former, the system has every chance to sample all possible multimolecular clusters in solution before selecting the one lowest in energy. These clusters would then aggregate to form larger clusters, but at each stage, the system is able to select that path which will minimize the energy. If some of these events lead to a local minimum, the system is able to correct itself and eventually find the global minimum. To paraphrase, we are speaking here of the thermodynamic crystal. In the chemical model, the individual interactions are all-important. Once a hydrogen bond forms between the strongest donor and acceptor, it cannot be undone, and the formation of the next hydrogen bond between the second donor and acceptor is inevitable. This is the kinetic crystal, or at least one of theAngew. Chem. Int. Ed. 2007, 46, 8342 8356
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Angewandtekinetic possibilities of crystallization. If crystallization is viewed as a supramolecular reaction, polymorphs are alternative reaction products (Figure 3). Two possibilities need to be considered during crystallization. In the first, the thermodynamic and kinetic outcomes of crystallization are identical; in other words, the crystal that is formed the fastest is always the most stable. In this case, it would normally not be possible to observe ambient-pressure polymorphism, however exhaustive the performed experimentation is. I have pointed out often in talks that compounds like benzoic acid, naphthalene, and d-glucose almost surely belong to this monomorphic category. In the second case, the kinetic form(s) is (are) different from the thermodynamic crystal, and polymorphs may, in principle, be observed with a greater or lesser degree of ease, provided adequate experimentation is carried out.[95, 96] This dichotomy can lead to some ambiguity. The crystal structures of decidedly monomorphic substances (such as the above-mentioned compounds) would seem to obey the geometrical or chemical models equally well. Polymorphic substances, on the other hand, would seem to follow either one or the other model, depending on which polymorph is selected. In effect, either or both models seem to be valid in different situations, leading to contradictions and statements to the effect that this or that model may or may not be correct.[8285, 9093] Only through a systematic study of polymorphic systems would it be possible to distinguish between kinetic and thermodynamic pathways during crystallization, and in effect to evaluate the chemical and geometrical models for a molecular crystal. Such studies are only just beginning to appear. In recent, important work Roy and Nangia have found that the hydrazone RSO2NHN=CR2 (R = p-tolyl) exists as three polymorphs and one pseudopolymorph. The most stable form, as determined by differential scanning calorimetry (DSC) and calculations, has the highest melting point (1608) but does not contain the best hydrogen bond, namely N HO=S. Indeed, the NH group is not hydrogen-bonded at all, not even to the weak p-ring acceptor in the molecule. Yet this form is more stable by 2.5 kcal mol1 than the polymorph nearest in energy, a kinetic form with the expected N HO=S hydrogen bond (synthon 4 in Scheme 2), and which converts to the stable thermodynamic form at about 1408. So, the best crystal packing does not always go with the best interactions. In another similar result, we found that the biphenyl aminophenol 5 (Scheme 2) exists as two conformational polymorphs. The kinetic form has the better interactions in terms of an infinite NHOHNHOH chain stabilized by cooperative effects. It is known that this infinite hydrogen-bonded chain is the most favored synthon for aminophenols. The more stable form has the better packing (by 1.5 kcal mol1) but has to make do with the less favorable OHO and NHN interactions. Alloxan is a more enigmatic case. No polymorphism has been reported for this compound, but the stable crystal structure is unusual in that a molecule which is very rich in NH donors and C=O acceptors does not form good NHO bonds in the solid state. The reason for this seems to be that a high-density, low-energy structure is possible with dipolar CO interactions such that strong hydrogen bonds may beAngew. Chem. Int. Ed. 2007, 46, 8342 8356
evaded. Commenting on this structure, I noted a few years ago that any way of minimizing the free energy is a respectable way. Dunitz and Schweizer have provided a quantitative rationalization of this structure in a recent publication, and they echo similar thoughts when they say that it is held together by whatever factors contribute to the cohesive energies. Alloxan also teaches us about the trade-off between close packing and directionality requirements of interactions. Dunitz and Schweizer note that although it has no conventional length hydrogen bonds perhaps even because of this?it has a higher density than any of the hypothetical structures with conventional hydrogen bonds, implying that such a trade-off between good interactions and good packing is important at least in some crystals. But in the end, one is tempted to suggest that the similarities between the geometrical and chemical models are more significant than the differences. To paraphrase informally, one joins closest-neighboring atoms in a crystal with dotted lines in the chemical model. But if one relaxes the criterion for joining the dots and draws a sufficiently large number of these dotted lines, one is back to the shape argument of the geometrical model. Reality probably lies somewhere in between, or maybe there is even no contradiction between these schools of thought. A major challenge is to establish general experimental protocols to obtain the thermodynamic crystal in any polymorphic system. This would mean finding methods to slow down nucleation, whether it be through high-temperature and hydrothermal experiments, gel growth, crystallization from supercritical fluids, or other methods still untried and unexplored. Obtaining the thermodynamic polymorph by brute-force methods could be difficult because crystallization is a kinetic phenomenon, and a kinetic polymorph could be locked in for years before one is even aware that there exists a more stable crystal form. This lesson came to us when we realized that the only form of 1,3,5-trinitrobenzene known for 125 years is a kinetic polymorph enabled through CHO interactions. This form is as much as 5.80 kcal mol1 less stable than the elusive thermodynamic form, which is threedimensionally close-packed and which was obtained only from ethyl acetate, and not even consistently at that. Being sure that a certain polymorph is the thermodynamic crystal is in itself a major breakthrough. In effect, it would mean proving that this particular crystal form has the lowest possible free energy in the structural landscapeand this would imply a very high degree of confidence in the various experimental and computational techniques that would be required. Incorporating both kinetic and thermodynamic possibilities, the supramolecular synthon concept provides a working blueprint for crystal design. I would like to reemphasize that synthons encapsulate features of both geometrical and chemical recognition. There is no stipulation that supramolecular synthons must contain hydrogen bonds or other directed interactions. They could just as well contain information of the mutual recognition of hydrocarbon fragments, such as rings and chains. Of course, the most optimal (that is, useful) synthon is a structural unit which condenses the maximum amount of information regarding molecular www.angewandte.org
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Reviewsrecognition into an entity of the minimum size. All models for the visualization of crystal structures use some method of simplification to generate smaller units which are hopefully representative of the complete crystal. The real question is, how much simplification is optimal, how much is insufficient, and how much is excessive? The geometrical model of Gavezzotti uses space group information to simplify the structure and generate smaller clusters of molecules; the purely chemical model of Etter uses only strong hydrogen bonds to reduce the crystal structure to its bare bones. The synthon model is another form of structural simplification, but it demands neither a scale of interaction energies, as does the chemical model, nor a scale of crystal packing energies, as does the geometrical model. It is purely probabilistic and is concerned only with the frequencies of occurrence of subjectively chosen but hopefully representative patterns in crystal structures. If a pattern is seen often enough, it is assumed to be (kinetically) favored and likely to recur in other crystal structures of related molecules. If a sufficiently large number of crystal structures are examined, any kind of molecule!crystal relationship may be predicted even if it is not understood entirely. Identifying a robust, or recurring, synthon does not presuppose any direct knowledge of the crystallization event, although indirect inferences may be drawn as discussed later in this review. The kinetic nature of crystallization, which arises from the high degrees of supersaturation that are generally involved, is the underlying reason and has so many conceptual similarities with covalentbond-making processes, which proceed often under kinetic control. The striking parallels that I drew between molecular and supramolecular synthons in my 1995 review are accordingly no surprise. They arise from the fact that one is comparing two kinetically controlled phenomena. Crystallization, then, is fundamentally different from the kinds of thermodynamically controlled supramolecular situations described by Whitesides in his 1995 review.
G. R. Desiraju
For rigid molecules containing only C, H, N, and O atoms (less than 20 non-H atoms) and with the number of symmetryindependent molecules in the crystal (Z) is 1, CSP generally gives the correct solution if the most stable form is the one which is also experimentally observed. With any relaxation of these conditions (flexible molecule, other elements present, greater than 20 non-H atoms, Z > 1, most stable form not observed experimentally), the problem quickly becomes extremely difficult to intractable.
5.1. Synthon-Based CSP When the kinetic form is the one obtained experimentally, we have suggested a knowledge-based alternative, the supramolecular synthon approach to CSP.[99, 108] In this methodology the computational results are biased manually with synthon information from a database of known crystal structures to incorporate the kinetic factors. Synthons in this database are loosely classified as small and large based on their complexity. The absence of a small synthon in a predicted structure is a negative factor and is justification for its down-ranking or elimination. The presence of a large synthon in a predicted structure is a positive factor and is grounds for its up-ranking. The highest ranked structures in this reranked list are taken as the predictions. We have shown that such synthon-based CSP (with the COM force field) works well for rigid aminophenols and related compounds. In this work, CSP was performed for nine aminohydroxy compounds (mostly substituted benzenes and naphthalenes; Scheme 3, right) with unknown crystal structures, using a training database of the 10 isomeric methylaminophenols and the three simple unsubstituted aminophenols (Scheme 3, left). Subsequent experimental verification of four of these predictions showed that two predictions were accurate (8-amino-2-naphthol, 4-aminocyclohexanol), one was somewhat acceptable in that the predicted synthons were found in the experimental packing (3-amino-2-naphthol), and one was incorrect (2-amino-4-ethylphenol). We assess these results as acceptable given the current scenario. Among all the problems associated with CSP, the most serious one seems to relate to molecular flexibility. The issue of conformational polymorphism has long been known. It is always difficult to anticipate the packing of a molecule when the molecular structure and the crystal structure influence one another implicitly. In the context of a computational exercise, how does one fix the molecular conformation before beginning a search of crystal space? Clearly molecular conformation and crystal packing cannot be varied simultaneously in the CSP protocol; the problem would quickly rise to unmanageable proportions. Some assumption is required regarding the molecular structure. Whether or not it is a correct assumption is not known before the CSP. In a recent study, Price and co-workers correctly predicted a second (and at that time unknown) form of aspirin. The assumption they made is that the unknown conformation is similar to the one in the known polymorph. This turns out to be a correct assumption, and all went well. However, if this were not the case, then the entire effort might well have been a failure. AAngew. Chem. Int. Ed. 2007, 46, 8342 8356
5. Crystal Structure Prediction (CSP)Crystal structure prediction (CSP) is the computational prediction, from the molecular structure, of the space group and the positional parameters of the atoms in the crystal structure.[95, 104] It is the most quantitative type of crystal engineering and is recognized to be a major scientific problem of great difficulty.[105, 106] A number of crystal structures are obtained computationally by using a selected force field, and the experimental structure is hidden generally amongst the 100 or so lowest-energy structures. When the experimental structure is also the thermodynamic structure, accurate force fields may reveal this structure as the global minimum. When the experimental structure is a higher-energy kinetic structure, a purely computational technique is often inadequate. CSP has been highlighted in a series of blind tests organized regularly since 2000 by the Cambridge Crystallographic Data Centre (CCDC) in which the participants are given a few (three and most recently four) molecular structures for each of which three solutions have to be deposited after a time period of around six months. The results have been mixed.
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Scheme 3. 13 training-set compounds (left) are used for the crystal structure prediction of nine aminophenols and related derivatives (right).
general strategy for the CSP of flexible molecules (say, two or three rotatable bonds) is a major challenge, and if successful would lead to considerable progress in crystal engineering in silico.
6. Crystallization MechanismsAt the heart of crystal engineering is the process of crystallization. As this process becomes better understood, crystal structure prediction will become more reliable, and in turn more effective control will be obtained over the design of both structure and function. Determining the mechanism of crystallization is the ultimate goal of crystal engineering and one of the outstanding problems in supramolecular sciences because the crystal is an emergent property of molecules. Crystallization is a supramolecular reaction. On the one side, there is the solution, which is an entropy-dominated situation. On the other, there is the crystal, which is the largely enthalpically determined outcome of the reaction. Between these must lie the crystal nucleus, which is possibly the highest energy point in the reaction coordinate. The path from solution to the nucleus represents an ever-changing balance between entropy and enthalpy, in favor of the latter. While very little is known about the actual course of events during crystallization, a plausible scenario may be sketched assuming that the nucleus lies somewhere along a smooth pathway from solution to crystal. As the elements of short-range order enter the immediate vicinity of the solute molecules, the solution rigidifies, gradually becoming a solutesolvent cluster. The point of nucleation may be likened to the transition state in a covalent-bond-making process, and is followed immediately by the exit of solvent into the bulk with the simultaneous formation of the crystal, a species which is characterized by long-range order. Just as it is nearly impossible to see a transition state directly, it will be correspondingly difficult to catch a crystal nucleus. It will not be easy to study crystal nucleation because crystallization is a non-equilibrium process which occurs under conditions of supersaturation (ofAngew. Chem. Int. Ed. 2007, 46, 8342 8356
solutions) or supercooling (of liquids). But the energies involved in a supramolecular reaction like crystallization are much smaller than those involved in typical covalent-bondmaking processes. Accordingly, it might be possible to draw some inferences about the crystallization mechanism from experiment. How this could be done is still an open question. Spectroscopy and crystallography, both of the normal and the time-resolved type, are possibilities.
6.1. Structures with Multiple Molecules in the Asymmetric Unit (Z > 1) An indirect way of observing the course of crystallization is offered by the study of crystal structures which contain multiple molecules in the crystallographic asymmetric unit (Z > 1). In the context of crystallization pathways, a crystal with Z > 1 could be a kinetic form which has been trapped before the molecules have adjusted themselves in their final orientations, which would be seen in a more stable form with Z = 1 (or a value less than in the kinetic form). This is an example of an interrupted crystallization, and the structure of this reaction intermediate could provide an approximation to the precursor crystal nucleus. Contributions in this regard have been made by Steed, who has referred to the high-Z structure as a fossil relic of the more stable crystal, and by Nangia, who has referred to these structures as snapshots of the crystallization reaction. We have noted this situation in two crystals, 6 and 7 (see Scheme 2). In pentafluorophenol (6) the more stable form with Z = 1 contains an infinite OHOHOHOH chain, the adjacent molecules being related by 21 symmetry. The Z = 3 structure is more interesting, being obtained in an in situ cryocrystallography experiment when an additive, pentafluoroaniline, is added. This structure contains finite trimer O HOHOH fragments, and we expect that it is an intermediate on the way to the infinite chain, with a concomitant synthon evolution towards the final structure (Figure 4). www.angewandte.org
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
G. R. Desiraju
structural descriptor of crystals. Accordingly, I do not use or advocate the use of terms like motif and pattern, which seem to be suggestive of the static crystal alone, as equivalents of synthon.
6.3. Late Stages of Crystallization To the extent that the nucleus lies on a smooth path between the solution and the crystal, its structure could be approximated as a liquid-like cluster which contains solute and solvent with some elements of order. However, most crystals of non-ionic organic compounds do not contain solvent. Accordingly, a characteristic occurrence during or just after nucleation would be the expulsion of solvent from the nucleus to the bulk solvent; this removal of solvent from the crystal is entropically advantageous and is possibly facile. Conversely, the retention of (ordered) solvent molecules in the crystal is evidence of enthalpic factors, notably the formation of strong hydrogen bonds between solute and solvent. According to such a model, the presence of solvent in a crystal could be taken as evidence of interrupted crystallization. The entropically facilitated expulsion of solvent from the crystal is countered by the enthalpic advantage that is gained from hydrogen bonding in retaining the solvent so that, in effect, the solvent is held by the crystal. If solvent expulsion is characteristic of completed crystallization, then solvent retention is evidence of incomplete or interrupted crystallization. Howard et al. have obtained evidence of such interruption in solvates of the alkyne diol 8 (Scheme 2), and their work highlights the late stages of crystallization when solvent is being expelled from the nascent crystal. Crystals were obtained both for the unsolvated diol and for the cyclooctylamine solvate. The compound belongs to the geminal alkynol family, for which synthons 9 and 10 (Scheme 2) are representative. The asymmetric unit of the solvate comprises two half molecules of the diol, each sitting on distinct inversion centers, together with one amine molecule (Scheme 4). The interaction hierarchies of the two diol molecules are distinctly different; while one of them is involved in forming synthon 9, the hydroxyl group of the other forms a strong OHN hydrogen bond with the amine. In doing so, it comes in
Figure 4. Orientation of pentafluorophenol (6) in the crystal (F green, C gray, O red, H blue). The structure with high Z (bottom) contains a fragment of the eventual infinite OHOH synthon seen in the structure above with Z = 1.
Similarly, the transformation of the higher-energy Z = 8 form of cyclohexane (7) into the more stable Z = 3 form was observed experimentally. Both forms have essentially the same packing, but there is a greater variation in conformations in the Z = 8 form. Accordingly, we have proposed that this is a case of symmetry evolution during crystallization.
6.2. Early Stages of Crystallization More direct glimpses of the events during crystallization are reported in recent studies from Davey, Howard, and ourselves. Davey and co-workers showed that the application of FT-IR spectroscopy to concentrated solutions of tetrolic acid shows a direct relationship between molecular self-association in solution and H-bonded patterns in the subsequently crystallized solid phases. Daveys work sheds light on the early stages of crystallization, because it involves measurements in solution. Tetrolic acid is notable in that it takes both the zero-dimensional dimer and one-dimensional catemer in its dimorphs. As mentioned in Section 1.2, the dimercatemer dichotomy is a classical problem in crystal engineering, and Daveys work is important in that it is the first evidence that the supramolecular synthons which are present in the final crystal have an existence in solution prior to crystallization. The metastable a form is obtained from CHCl3 and contains the dimer. The stable b form is catemeric and is obtained from ethanol. Fortunately, some IR spectral features of the two forms are non-overlapping, and it is possible to unequivocally assign some peaks to just one or the other of the forms, leading to the above-mentioned result. This result is far-reaching and shows that the synthon is a structural unit of significance in all stages of crystallization, from solution, to aggregation, nucleation, and finally growth. The synthon is of mechanistic significance and not merely a
Scheme 4. Interruption of synthon formation by solvent. Cyclooctylamine (RNH2) forms a hydrogen bond with a hydroxy group in alkynol 8, preventing the formation of synthon 10. Synthon 9 is formed as usual. Without such interruption, synthons 9 and 10 would be formed in their usual fused manner as seen in Figure 2 for alkynols 2 and 3.Angew. Chem. Int. Ed. 2007, 46, 8342 8356
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Angewandtebetween two ethynyl groups and intervenes in the formation of synthon 10. As a result of this, the ethynyl H atom remains free. However, the orientation of the ethynyl groups is closely reminiscent of both the cooperative synthons 9 and 10, which are the hallmarks of the geminal alkynol family; only in the solvate these groups are obstructed and separated by the steric bulk of the cyclooctylamine. In other words, this is the closest example of what could be imagined as the interruption of a representative synthon (in this case, 10) by the formation of a strong OHN bond from the solvent. The presence of two relatively weak NHp (2.96 , 3.15 ) interactions could be rationalized as bringing the structure one step closer to the crystallization point, when solvent extrusion from the bulk occurs and a solute-rich structure results. sac , Na+ (some of which is not necessarily hexacoordinated), and water (some of which is ill-resolved). Notably, there is a variation in the occupancies of these species between crystal to crystal and possibly between one temperature and another. All in all, we carried out structure determinations of four crystals at four different temperatures (total of eight data sets). The overall conclusion is that there is appreciable mobility of the species in the irregular region, and it may be taken to be in a state of incipient crystallization. The third unusual feature is that dihydrate 11 can exist in equilibrium with water. When a crystal is placed in the proximity of a single drop of water in a closed environment, it absorbs water rapidly. Further exposure to the vapor results in dissolution, which is followed by rapid recrystallization if the watersaturated environment is removed. All of this, when taken with the presence of the irregular disordered domains, indicates a crystal that is very close to the dissolution point. We note further that the solubility of 11 at 27 8C is 120 g in 100 g water, which is equivalent to a water content just seven times less than the saturated solution. The fourth feature of note is that crystals of 11 also lose water readily. Remarkably, a solid that is deliquescent in a water-rich environment is efflorescent in a water-poor environment, and water loss occurs in two stages. The first stage begins as low as 35 8C and is essentially complete by 50 8C to yield the lower hydrate 12, the structure of which is shown in Figure 6. The second stage occurs between 100 8C and 115 8C and leads to the anhydrate.
6.4. Intermediate Stages of Crystallization. Catching the Nucleus The early stage of crystallization involves the first synthon formation in solution while the late stage involves solvent expulsion. The intermediate stage of crystallization is in many ways the most fascinating because it may be that it is during this stage that nucleation occurs. We recently determined the crystal structure of sodium saccharin dihydrate, Na(sac)(H2O)1.875 (11) and showed that this heavily hydrated structure is a very good model for the nucleus of the lower hydrate Na3(sac)3(H2O)2 (12). Indeed this complex structure is akin to a metastable high-energy intermediate, and for a number of reasons, we have argued that it is as good a model for a crystal nucleus as can be obtained presently. The structure of dihydrate 11 is shown in Figure 5 and has several unusual features. The first is the large unit cell (15 614 3, P21/n, Z = 4). With 64 Na+ ions, 64 sac ions, and 120 water molecules in the unit cell, this structure is one of the largest and most complex ever for ions/molecules that are as small and simple as these. The second feature is that a part of it, the regular region, resembles a conventional crystal, but an adjacent part, the irregular region, has solution-like characteristics. In the former domain, the saccharinate anions are nearly parallel and stacked, the Na+ ions are hexacoordinated with water and sac , and the water molecules are efficiently hydrogen-bonded. In the irregular region, there is disorder of
Figure 6. Crystal structure of the lower hydrate, (Na)3(sac)3(H2O)2 (12; Na purple, S yellow, O red, N blue, C gray, H light blue), obtained from dihydrate 11 by loss of water. Note that the residues stacked perpendicular to the plane of the page are related to the ordered regions in the dihydrate structure.
Figure 5. Crystal structure of the asymmetric unit of sodium saccharin dihydrate, Na(sac)(H2O)1.875 (11; Na purple, S yellow, O red, N blue, C gray, H beige). Notice the ordered (left) and disordered (right) regions of the crystal with five and three saccharin dimers, respectively. The latter region is in a state of incipient crystallization.Angew. Chem. Int. Ed. 2007, 46, 8342 8356
Inspection of the crystal structures of 11 and 12 shows that while the sac residues in 11 are all nearly parallel, those in 12 occur in two groups that are perpendicular to each another. The stacking of residues in the infinite stack down  bears a close resemblance to that in the regular domains of hydrate 11. The residues that occur as discrete dimers in 12, perpendicular to the infinite stack, are in a stoichiometry that is half that of the residues in the infinite stack. This 2:1 stoichiometry of residues in 12 is reminiscent of the 5:3 demarcation of sac residues in the regular and irregular www.angewandte.org
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Reviewsregions of dihydrate 11, and is suggestive of a possible mechanism for the 11!12 conversion. While the regular domains are largely conserved, the residues in the irregular domains might move into the empty regions created by the loss of water, and also assume a perpendicular geometry. This mechanism is reasonable because maximum movement of residues occurs in those regions of 11 where the arrangement is the least regular and where molecular motion is already expected to be facile. Additionally, selected supramolecular synthons in dihydrate 11 are retained in hydrate 12. The stacked synthons in the regular domains of 11 are preserved as mentioned above. Hydrogen-bonded synthons in the irregular domains of 11 are also conserved in 12. The fact that these synthons are carried over into 12 even as there is much structural reorganization is in keeping with the idea of synthons as kinetically significant units that are preserved through all stages of crystallization. The unusual features in the structure of 11 argue that it is a good model for nucleation in the crystallization of the hydrate 12 from water. A large unit cell, in itself, is not exceptional, but for crystals wherein the building blocks (molecules, ions, solvent) are so small, such a large unit cell is noteworthy. The combination of the large cell, with regular and irregular domains, and also the excessive amount of solvent in the crystal are very suggestive of a crystallization reaction still in progress. Indeed, dihydrate 11 seems to be evenly poised between solution and hydrate 12. There is no other reported example of a substance that gains and loses solvent so easily, and there is not much difference in water content between crystalline 11 and the saturated solution. Amazingly, the same compound loses water at 35 8C, and the resulting hydrate 12 does not gain water when exposed to the vapor. Easy water gain or loss is, in itself, unexceptional. When it occurs for the same substance, it becomes significant and suggests that 11 is a high-energy intermediate which bridges the saturated solution and the stable hydrate 12. In keeping with the idea of crystallization as a supramolecular reaction and the description of dihydrate 11 as a supramolecular transition state, one can apply the Hammond postulate and conclude that 11 is an example of a late transition state. Large regions of 11 resemble that of 12, and there are no waterwater interactions. The elements of order have well entered the crystal nucleus, the important supramolecular synthons are in place (if not exactly in the correct locations), and the product of crystallization (hydrate 12) is a kinetic product. It is still a matter of conjecture that crystal nuclei which are early transition states will have solution-like character, and that they will lead to thermodynamic products (perhaps the anhydrate).
G. R. Desiraju
some of the difficult questions posed in this review will yield their secrets only with the application of sophisticated experimental methods, which can make measurements in very small distances and time scales. As a type of synthetic activity it offers considerable scope for artistry and imagination, both of which are bounded only by human ingenuity. But above all, it is the conceptual challenges in understanding the crystal and crystallization that strain the limits of the chemical researcher because crystal engineering is a study of systems that are both diverse and complex. I thank the Department of Science and Technology, Government of India, for support of my research and exchange programs over the years. This article was first conceived as a chalk-and-blackboard talk delivered at the Indaba 5 conference Models, Mysteries and Magic of Molecules held at Berg-en-dal, Kruger National Park, South Africa (August 20 25, 2006).Received: February 6, 2007 Published online: September 27, 2007
7. Summary and OutlookI have tried to sketch some current themes in a discipline that has crossed the threshold between a developing and mainstream activity. Crystal engineering has much to offer the chemist because it is mechanistic, synthetic, and conceptual in its theme. As a mechanistic subject, there are considerable opportunities for the use of instrumental techniques. Indeed,
 G. R. Desiraju, Crystal Engineering. The Design of Organic Solids, Elsevier, Amsterdam, 1989.  Solid State Photochemistry. A Collection of Papers by G. M. J. Schmidt and his Collaborators (Monographs in Modern Chemistry, Vol. 8) (Ed.: D. Ginsburg), Verlag Chemie, Weinheim, 1976.  A. I. Kitaigorodskii, Molecular Crystals and Molecules, Academic Press, New York, 1973.  J. M. Thomas, Nature 1981, 289, 633 634.  L. Addadi, M. Lahav, Pure Appl. Chem. 1979, 51, 1269 1284.  G. Wegner, Z. Naturforsch. B 1969, 24, 824 832.  Crystal Engineering. From Molecules and Crystals to Materials (Eds.: D. Braga, F. Grepioni, A. G. Orpen), Kluwer, Dordrecht, 1999.  Frontiers in Crystal Engineering (Eds.: E. R. Tiekink, J. J. Vittal), Wiley, Chichester, 2005.  Crystal Design. Structure and Function. Perspectives in Supramolecular Chemistry (Ed.: G. R. Desiraju), Wiley, Chichester, 2003.  M. Eddaoudi, D. B. Moler, H. L. Li, B. L. Chen, T. M. Reinecke, M. OKeeffe, O. M. Yaghi, Acc. Chem. Res. 2001, 34, 319 330.  B. Moulton, M. J. Zaworotko, Chem. Rev. 2001, 101, 1629 1658.  A. Nangia, G. R. Desiraju, Acta Crystallogr. Sect. A 1998, 54, 934 944.  C. B. Aakery, Acta Crystallogr. Sect. B 1997, 53, 569 586.  M. W. Hosseini, Acc. Chem. Res. 2005, 38, 313 323.  O. R. Evans, W. B. Lin, Acc. Chem. Res. 2002, 35, 511 522.  I. Goldberg, Chem. Commun. 2005, 1243 1254.  J. D. Wuest, Chem. Commun. 2005, 5830 5837.  M. D. Ward, Chem. Commun. 2005, 5838 5842.  C. V. K. Sharma, Cryst. Growth Des. 2002, 2, 465 474.  D. Braga, F. Grepioni, Chem. Commun. 2005, 3635 3645.  A. D. Burrows, Encyclopedia of Supramolecular Chemistry, Vol. 1 (Eds.: J. Atwood, J. Steed), Marcel Dekker, New York, 2004, pp. 319 325.  P. Coppens, S. L. Zheng, M. Gembicky, M. Messerschmidt, P. M. Dominiak, CrystEngComm 2006, 8, 735 741.  R. Bishop, Synlett 1999, 1351 1358.  K. Biradha, CrystEngComm 2003, 5, 374 384.Angew. Chem. Int. Ed. 2007, 46, 8342 8356
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Angewandte S. A. Dalrymple, G. K. H. Shimizu, J. Mol. Struct. 2006, 796, 95 106.  P. Erk, H. Hengelsberg, M. F. Haddow, R. van Gelder, CrystEngComm 2004, 6, 474 483.  J. M. Lehn, Angew. Chem. 1988, 100, 91 116; Angew. Chem. Int. Ed. Engl. 1988, 27, 89 112.  J. D. Dunitz, Pure Appl. Chem. 1991, 63, 177 185.  G. M. Whitesides, E. E. Simanek, J. P. Mathias, C. T. Seto, D. N. Chin, M. Mammen, D. M. Gordon, Acc. Chem. Res. 1995, 28, 37 44.  G. R. Desiraju, Angew. Chem. 1995, 107, 2541 2558; Angew. Chem. Int. Ed. Engl. 1995, 34, 2311 2327.  The less valid this assumption, the less useful is the concept of the supramolecular synthon in crystal engineering. It is recognized that any crystal structure is complex, and that its analysis into smaller units is, of necessity, a simplification. The question, however, is whether or not a particular simplification affects ones comprehension of a structure to such an extent that one is unable to go back in a synthetic step and regenerate a crystal structure of a related molecule. Alternatively, if the simplification is very slight, there is no real advantage gained in invoking the synthon. Accordingly, the supramolecular synthon approach to crystal engineering hinges on whether or not a particular simplification (structure to synthon) is substantial enough to allow its easy use in a subsequent synthetic step (synthon to structure), but not so excessive that essential attributes of a structure are lost in the process of simplification, rendering subsequent crystal engineering unreliable.  M. C. T. Fyfe, J. F. Stoddart, Acc. Chem. Res. 1997, 30, 393 401.  N. Takeda, K. Umemoto, K. Yamaguchi, M. Fujita, Nature 1999, 398, 794 796.  V. Maurizot, M. Yoshizawa, M. Kawano, M. Fujita, Dalton Trans. 2006, 2750 2756.  S. R. Seidel, P. J. Stang, Acc. Chem. Res. 2002, 35, 972 983.  D. L. Caulder, K. N. Raymond, Acc. Chem. Res. 1999, 32, 975 982.  B. J. Holliday, C. A. Mirkin, Angew. Chem. 2001, 113, 2076 2097; Angew. Chem. Int. Ed. 2001, 40, 2022 2043.  A. R. Williams, B. H. Northrop, T. Chang, J. F. Stoddart, A. J. P. White, D. J. Williams, Angew. Chem. 2006, 118, 6817 6821; Angew. Chem. Int. Ed. 2006, 45, 6665 6669.  G. R. Desiraju, Curr. Sci. 2005, 88, 374 380.  D. Das, G. R. Desiraju, Chem. Asian J. 2006, 1, 231 244.  S. S. Kuduva, D. C. Craig, A. Nangia, G. R. Desiraju, J. Am. Chem. Soc. 1999, 121, 1936 1944.  J. Bernstein, Polymorphism in Molecular Crystals, Clarendon, Oxford, 2002.  J. Bernstein, Chem. Commun. 2005, 5007 5012.  S. Datta, D. J. W. Grant, Nat. Rev. Drug Discovery 2004, 3, 42 57.  . Almarsson, M. J. Zaworotko, Chem. Commun. 2004, 1889 1896.  O. Ermer, J. Am. Chem. Soc. 1988, 110, 3747 3754.  S. R. Batten, R. Robson, Angew. Chem. 1998, 110, 1558 1595; Angew. Chem. Int. Ed. 1998, 37, 1460 1494.  R. Thaimattam, C. V. K. Sharma, A. Clearfield, G. R. Desiraju, Cryst. Growth Des. 2001, 1, 103 106.  R. Banerjee, R. Mondal, J. A. K. Howard, G. R. Desiraju, Cryst. Growth Des. 2006, 6, 999 1009.  S. Kitagawa, R. Kitaura, S. Noro, Angew. Chem. 2004, 116, 2388 2430; Angew. Chem. Int. Ed. 2004, 43, 2334 2375.  L. Carlucci, G. Ciani, D. M. Proserpio, Coord. Chem. Rev. 2003, 246, 247 289.  G. Frey, C. Mellot-Draznieks, C. Serre, F. Millange, Acc. Chem. Res. 2005, 38, 217 225.  N. R. Champness, Dalton Trans. 2005, 877 880.Angew. Chem. Int. Ed. 2007, 46, 8342 8356
 B. F. Hoskins, R. Robson, J. Am. Chem. Soc. 1990, 112, 1546 1554.  O. M. Yaghi, M. OKeeffe, N. W. Ockwig, H. K. Chae, M. Eddaoudi, J. Kim, Nature 2003, 423, 705 714.  J. L. C. Rowsell, O. M. Yaghi, Angew. Chem. 2005, 117, 4748 4758; Angew. Chem. Int. Ed. 2005, 44, 4670 4679.  R. Matsuda, R. Kitaura, S. Kitagawa, Y. Kubota, R. V. Belosludov, T. C. Kobayashi, H. Sakamoto, T. Chiba, M. Takata, Y. Kawazoe, Y. Mita, Nature 2005, 436, 238 241.  Y. Kubota, M. Takata, R. Matsuda, R. Kitaura, S. Kitagawa, T. C. Kobayashi, Angew. Chem. 2006, 118, 5054 5058; Angew. Chem. Int. Ed. 2006, 45, 4932 4936.  G. R. Desiraju, T. Steiner, The Weak Hydrogen Bond in Structural Chemistry and Biology, OUP, Oxford, 1999.  T. Steiner, Angew. Chem. 2002, 114, 50 80; Angew. Chem. Int. Ed. 2002, 41, 48 76.  J. D. Dunitz, A. Gavezzotti, Angew. Chem. 2005, 117, 1796 1819; Angew. Chem. Int. Ed. 2005, 44, 1766 1787.  J. M. Robertson, Organic Crystals and Molecules, Cornell University, Ithaca, 1953, p 239. Another generalization derived from a study of these various crystal structures is what might be termed the principle of maximum hydrogen bonding. All available hydrogen atoms, attached to the electronegative groups, are generally employed in hydrogen bond formation.  T. Steiner, G. Koellner, J. Mol. Biol. 2001, 305, 535 557.  G. A. Jeffrey, Introduction to Hydrogen Bonding, OUP, Oxford, 1997.  D. Braga, F. Grepioni, G. R. Desiraju, Chem. Rev. 1998, 98, 1375 1405.  L. Brammer, Chem. Soc. Rev. 2004, 33, 476 489.  P. Vishweshwar, N. J. Babu, A. Nangia, S. A. Mason, H. Puschmann, R. Mondal, J. A. K. Howard, J. Phys. Chem. 2004, 108, 9406 9416.  W. Zierkiewicz, P. Jurecka, P. Hobza, ChemPhysChem 2005, 6, 609 617.  A. Angeloni, P. C. Crawford, A. G. Orpen, T. J. Podesta, B. J. Shore, Chem. Eur. J. 2004, 10, 3783 3791.  D. B. Leznoff, B. Y. Xue, R. J. Batchelor, F. W. B. Einstein, B. O. Patrick, Inorg. Chem. 2001, 40, 6026 6034.  A. A. Borkowski, C. L. Cahill, Cryst. Growth Des. 2006, 6, 2241 2247, and the succeeding paper.  Z. F. Zhou, K. D. M. Harris, ChemPhysChem 2006, 7, 1649 1653.  J. D. Dunitz, R. Taylor, Chem. Eur. J. 1997, 3, 89 98.  V. R. Thalladi, H. C. Weiss, D. Blser, R. Boese, A. Nangia, G. R. Desiraju, J. Am. Chem. Soc. 1998, 120, 8702 8710.  I. Hyla-Kryspin, G. Haufe, S. Grimme, Chem. Eur. J. 2004, 10, 3411 3422.  K. Reichenbcher, H. I. Suss, J. Hulliger, Chem. Soc. Rev. 2005, 34, 22 30.  O. Jeannin, M. Fourmigu, Chem. Eur. J. 2006, 12, 2994 3005.  J. A. Gladysz, D. P. Curran, Tetrahedron 2002, 58, 3823 3825.  P. Ganguly, J. Am. Chem. Soc. 1993, 115, 9287 9288.  S. C. F. Kui, N. Y. Zhu, M. C. W. Chan, Angew. Chem. 2003, 115, 1666 1670; Angew. Chem. Int. Ed. 2003, 42, 1628 1632.  F. Hof, F. Diederich, Chem. Commun. 2004, 484 487.  J. D. Dunitz, A. Gavezzotti, Acc. Chem. Res. 1999, 32, 677 684.  F. Demartin, G. Filippini, A. Gavezzotti, S. Rizzato, Acta Crystallogr. Sect B 2004, 60, 609 620.  J. D. Dunitz, A. Gavezzotti, Cryst. Growth Des. 2005, 5, 2180 2189.  J. D. Dunitz, B. Schweizer, CrystEngComm 2007, 9, 266 269.  In his book (reference , p. 85), Kitaigorodskii writes that so far only one significant conclusion suggests itself: The formation of hydrogen bonds does not handicap the layout of molecules in conformity with the general [geometrical] rules of
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Reviewsthe packing of crystals. About molecular compounds (cocrystals in modern-day parlance) he says the formation of such a crystal does not necessarily point to some kind of specific forces between the compound molecules. This is all he is willing to concede! T. Steiner, G. R. Desiraju, Chem. Commun. 1998, 891 892. A. J. Pertsin, A. I. Kitaigorodskii, The Atom-Atom Potential Method, Springer, Berlin, 1987, p. 3. M. C. Etter, Acc. Chem. Res. 1990, 23, 120 126. C. B. Aakery, D. J. Salmon, CrystEngComm 2005, 7, 439 448, and references therein. P. Vishweshwar, A. Nangia, V. M. Lynch, Cryst. Growth Des. 2003, 3, 783 790. P. W. Baures, J. R. Rush, A. V. Wiznycia, J. Desper, A. A. Helfrich, A. M. Beatty, Cryst. Growth Des. 2002, 2, 653 664. J. F. Remenar, S. L. Morissette, M. L. Peterson, B. Moulton, J. M. MacPhee, H. R. Guzman, . Almarsson, J. Am. Chem. Soc. 2003, 125, 8456 8457. By directionality in this context is meant any kind of spatial or chemical anisotropy in the crystal structure. G. R. Desiraju, Nat. Mater. 2002, 1, 77 79. It is unfortunate that McCrones dictum has been overused to the point where some chemists believe that any organic compound will give (ambient-pressure) polymorphs, provided enough time and money is spent in this enterprise. See, W. C. McCrone, Physics and Chemistry of the Organic Solid State, Vol. 2 (Eds.: D. Fox, M. M. Labes, A. Weissberger), Wiley Interscience, New York, 1965, pp. 725 767. It is at least this authors opinion that every compound has different polymorphic forms and that, in general, the number of forms known for a given compound is proportional to the time and money spent in research on that compound. I would like to suggest that this dictum is true only in those cases where the kinetic outcome of crystallization is distinct from the thermodynamic one. S. Roy, A. Nangia, Cryst. Growth Des. 2007, 7, DOI: 10.1021/ cg070542t. A. Dey, G. R. Desiraju, CrystEngComm 2006, 8, 478 482. A. Dey, M. T. Kirchner, V. R. Vangala, G. R. Desiraju, R. Mondal, J. A. K. Howard, J. Am. Chem. Soc. 2005, 127, 10545 10559. K. Mller, F. Diederich, R. Paulini, Angew. Chem. 2005, 117, 1820 1839; Angew. Chem. Int. Ed. 2005, 44, 1788 1805. G. R. Desiraju, CrystEngComm 2002, 4, 499. P. K. Thallapally, R. K. R. Jetti, A. K. Katz, H. L. Carrell, K. Singh, K. Lahiri, S. R. Kotha, R. Boese, G. R. Desiraju, Angew. Chem. 2004, 116, 1169 1175; Angew. Chem. Int. Ed. 2004, 43, 1149 1155.
G. R. Desiraju
      
  
  
  
 T. Gelbrich, M. B. Hursthouse, CrystEngComm 2005, 7, 324 336. These authors distinguish between supramolecular synthons and their so-called supramolecular constructs and state that synthons contain well-defined directional interactions as opposed to constructs. My original definition of the term supramolecular synthon (reference ) neither contains nor implies any such limitation. The term synthon includes all types of molecular recognition. Given in my 1995 review are examples of synthons which contain only van der Waals and other largely nondirectional interactions (phenylphenyl herringbone and stacking, alkylalkyl),  J. D. Dunitz, Chem. Commun. 2003, 545 548.  A. R. Oganov, C. W. Glass, J. Chem. Phys. 2006, 124, 244704.  P. Raiteri, R. Martonak, M. Parrinello, Angew. Chem. 2005, 117, 3835 3839; Angew. Chem. Int. Ed. 2005, 44, 3769 3773.  G. M. Day, W. D. S. Motherwell, H. L. Ammon, S. X. M. Boerrigter, R. G. Della Valle, E. Venuti, A. Dzyabchenko, J. D. Dunitz, B. Schweizer, B. P. van Eijk, P. Erk, J. C. Facelli, V. E. Bazterra, M. B. Ferraro, D. W. M. Hofmann, F. J. J. Leusen, C. Liang, C. C. Pantelides, P. G. Karamertzanis, S. L. Price, T. C. Lewis, H. Nowell, A. Torrisi, H. A. Scheraga, Y. A. Arnautova, M. U. Schmidt, P. Verwer, Acta Crystallogr. Sect. B 2005, 61, 511 527.  J. A. R. P. Sarma, G. R. Desiraju, Cryst. Growth Des. 2002, 2, 93 100.  A. Dey, N. N. Pati, G. R. Desiraju, CrystEngComm 2006, 8, 751 755.  C. Ouvrard, S. L. Price, Cryst. Growth Des. 2004, 4, 1119 1127.  G. R. Desiraju, CrystEngComm 2007, 9, 91 92.  J. W. Steed, CrystEngComm 2003, 5, 169 179.  V. S. S. Kumar, A. Addlagatta, A. Nangia, W. T. Robinson, C. K. Broder, R. Mondal, I. R. Evans, J. A. K. Howard, F. H. Allen, Angew. Chem. 2002, 114, 4004 4007; Angew. Chem. Int. Ed. 2002, 41, 3848 3851.  D. Das, R. Banerjee, R. Mondal, J. A. K. Howard, R. Boese, G. R. Desiraju, Chem. Commun. 2006, 555 557; see also: M. Gdaniec, CrystEngComm 2007, 9, 286 288. However, we stand by our result on the isolated trimer polymorph of pentafluorophenol, and will submit our rebuttal shortly (D. Blser, M. T. Kirchner, R. Boese, G. R. Desiraju, in preparation).  R. J. Davey, G. Dent, R. K. Mughal, S. Parveen, Cryst. Growth Des. 2006, 6, 1788 1796.  R. Mondal, J. A. K. Howard, R. Banerjee, G. R. Desiraju, Cryst. Growth Des. 2006, 6, 2507 2516.  R. Banerjee, P. M. Bhatt, M. T. Kirchner, G. R. Desiraju, Angew. Chem. 2005, 117, 2571 2576; Angew. Chem. Int. Ed. 2005, 44, 2515 2520.  A. Nangia, G. R. Desiraju, Chem. Commun. 1999, 605 606.
2007 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim
Angew. Chem. Int. Ed. 2007, 46, 8342 8356